#------------------------------------------------------------------------------
#$Date: 2024-05-23 12:45:01 +0300 (Thu, 23 May 2024) $
#$Revision: 292002 $
#$URL: file:///home/coder/svn-repositories/cod/cif/9/01/37/9013703.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the American Mineralogist Crystal Structure Database,
# http://rruff.geo.arizona.edu/AMS/amcsd.php
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_9013703
loop_
_publ_author_name
'De Villiers, J. P. R.'
'Liles, D. C.'
_publ_section_title
;
 The crystal-structure and vacancy distribution in 6C pyrrhotite
 Locality: Mponeng Mine, South Africa
 Note: coordinate of S7 altered to match reported bond lengths
;
_journal_name_full               'American Mineralogist'
_journal_page_first              148
_journal_page_last               152
_journal_paper_doi               10.2138/am.2010.3266
_journal_volume                  95
_journal_year                    2010
_chemical_formula_sum            'Fe2.747 Ni0.253 S3'
_chemical_name_mineral           Pyrrhotite
_symmetry_space_group_name_H-M   'F 1 d 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.003
_cell_angle_gamma                90
_cell_length_a                   6.8973
_cell_length_b                   11.954
_cell_length_c                   34.521
_cell_formula_units_Z            32
_cell_volume                     2846.268
_exptl_crystal_density_diffrn    4.937
_cod_original_formula_sum        'Fe2.747 Ni.253 S3'
_cod_database_code               9013703
loop_
_symmetry_equiv_pos_as_xyz
x,y,z
x,1/2+y,1/2+z
1/2+x,y,1/2+z
1/2+x,1/2+y,z
1/4+x,-y,1/4+z
1/4+x,1/2-y,3/4+z
3/4+x,-y,3/4+z
3/4+x,1/2-y,1/4+z
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_U_iso_or_equiv
Fe1 0.13600 0.12960 0.00020 1.00000 0.02800
Fe2 0.11540 0.13240 0.08400 1.00000 0.02300
Fe3 0.14510 0.11280 0.16680 1.00000 0.01900
Fe4 0.11730 0.12880 0.25070 1.00000 0.02900
Fe5 0.11620 0.12910 0.33510 1.00000 0.01800
Fe6 0.13950 0.12410 0.41930 0.89800 0.02600
Ni6 0.13950 0.12410 0.41930 0.10200 0.02600
Fe7 0.11960 0.12230 0.50340 0.66100 0.02800
Ni7 0.11960 0.12230 0.50340 0.33900 0.02800
Fe8 0.14210 0.12920 0.58100 0.55600 0.01500
Ni8 0.14210 0.12920 0.58100 0.44400 0.01500
Fe9 0.10960 0.12310 0.66490 1.00000 0.02200
Fe10 0.13250 0.12200 0.75010 1.00000 0.02600
Fe11 0.13630 0.13530 0.83350 0.87400 0.01800
Ni11 0.13630 0.13530 0.83350 0.12600 0.01800
Fe12 0.11510 0.11250 0.91640 1.00000 0.02000
S1 0.37610 0.04080 -0.04220 1.00000 0.01000
S2 0.37560 0.04080 0.12150 1.00000 0.01200
S3 0.37810 0.04190 0.29260 1.00000 0.01200
S4 0.37780 0.04170 0.46100 1.00000 0.01600
S5 0.37620 0.04150 0.62570 1.00000 0.01400
S6 0.37520 0.04330 0.79250 1.00000 0.01100
S7 0.37500 0.20750 0.04260 1.00000 0.01300
S8 0.37880 0.20760 0.20960 1.00000 0.01400
S9 0.37530 0.20840 0.37520 1.00000 0.00900
S10 0.37820 0.21000 0.54010 1.00000 0.01300
S11 0.37700 0.20790 0.70570 1.00000 0.01400
S12 0.37560 0.20850 0.87820 1.00000 0.01100
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0005000
